Toward three-dimensionally ordered nanoporous graphene materials: template synthesis, structure, and applications

Precise template synthesis will realize three-dimensionally ordered nanoporous graphenes (NPGs) with a spatially controlled seamless graphene structure and fewer edges. These structural features result in superelastic nature, high electrochemical stability, high electrical conductivity, and fast diffusion of gases and ions at the same time. Such innovative 3D graphene materials are conducive to solving energy-related issues for a better future. To further improve the attractive properties of NPGs, we review the template synthesis and its mechanism by chemical vapor deposition of hydrocarbons, analysis of the nanoporous graphene structure, and applications in electrochemical and mechanical devices.


Introduction
Carbon materials have industrial applications owing to their excellent features such as electrical conductivity, chemical and thermal stability, light weight, and low cost of preparation. 1 Nevertheless, the actual structures of carbon materials have not been well documented until recently, except for their chemical composition.Recent developments in analytical technologies for probing the structure of carbon materials, such as transmission electron microscopy, [2][3][4] Raman spectroscopy, [5][6][7] and high-sensitivity temperature-programmed desorption methods, 8,9 have enabled understanding of the actual threedimensional (3D) structure of carbon materials at the molecular and atomic levels.
With the developed tools for nanoscale analysis, the synthesis and understanding of nanostructured carbon materials have further expanded their elds and applications.1][22][23][24] Consequently, many advanced carbon materials, including carbon bers, carbon nanotubes (CNTs), graphenes, structural graphite, and carbon foams have been developed with improved physicochemical properties, and they are growing at a compound average growth rate (CAGR) of ∼6% with an annual global market of 3 billion USD in 2015. 25They are extensively used as adsorbents, 26 catalysts, [27][28][29][30][31][32][33] catalyst supports, 34 conductive additives, [35][36][37] and anode materials 38 in batteries, supercapacitors, 39,40 polymerelectrolyte fuel cells (PEFCs), 41 and photothermal conversion. 42n this context, the chemical science of two-dimensional (2D) graphene and its zero-dimensional (0D) and one-dimensional (1D) analogs has been extensively studied in recent decades.5][46][47][48] Single-plate graphene materials have high electrical conductivity and high thermal/ chemical stability; therefore, they are suitable for practical applications in energy-related devices.A class of 1D-graphene, carbon nanotubes 49,50 and cylindrical analogs, 51 has also been investigated for electrochemical and catalysis applications owing to their high electrical conductivity. 52 challenging aspect is the synthesis of the corresponding 3D graphene materials [53][54][55] from a 2D scaffold. 13Reducing the dimension of 2D graphene can be used to develop 3D graphene; the 0D analog of the fullerene family, 56 a good electron acceptor, 57 can be used as a building block to develop 3Danalogs. 58Catalytic carbonization has also been successfully applied to prepare 3D graphene architecture. 23,29,59However, the precise synthesis of 3D-ordered graphene materials with well-dened negatively curved 3D networks 60,61 remains an emerging topic since British scientists predicted imaginary carbon frameworks with 8-membered rings in hexagons to achieve a 3D structure with low strain. 53These materials are highly symmetric and possess highly ordered nanostructures that provide various fascinating functions (vide infra).For example, material surfaces for the adsorption of gases should be as homogeneous as possible with respect to the structure and chemical composition 62 for better and faster reactions, and imaginary 3D-ordered carbon frameworks should meet these criteria.The novel electronic nature of these frameworks makes them appealing for various applications.
In this review, we provide an overview of recent progress in the synthesis, structural characterization, and application of electrochemical and mechanical devices of 3D-ordered porous graphene material nanostructures.The remainder of this paper is organized as follows: in Section 2, we discuss typical synthetic procedures using templating carbonization on nanostructured precursor materials, such as zeolite and alumina.We then focus on the reaction mechanism of the carbon growth mechanism of CH 4 -CVD on alumina and the structure of the resultant 3D graphene, directed toward achieving a periodically ordered graphene nanostructure (Fig. 1).In Section 3, we provide an overview of how the 3D continuous nature of porous graphene drives its potential applications in electric double-layer capacitors, next-generation Li-ion batteries, and refrigeration devices based on mechanical force.In Section 4, we summarize this review and describe our outlook for further fundamental and application studies on 3D-ordered graphenes in the near future.

Synthesis and structure of templated carbons
A template method (alias dictus nanocasting) 63 has been explored for the synthesis of well-dened nanostructured materials.The chemical and physical properties of the obtained nanomaterials can be tuned by using the synthesis procedure as well as the precursor materials, 2 and CVD is a powerful method to precisely control nanostructures at the atomic level. 64For example, Ito and co-workers reported sophisticated macroporous (>50 nm) 3D graphene materials using CVD of benzene on a porous Ni template. 23The material maintains the electronic nature of pristine 2D graphene, and its analogs with structural defects, including substitutional defects and adatoms of nitrogen and sulfur, work efficiently as catalysts. 28,29,65wing to their high electrical conductivity.Recently, the effects of structural topology 66,67 and mechanical 68 and electronic properties 69 have also been well studied.Thus, these materials are excellent candidates for developing ideal 3D graphene materials.However, we recognized that a 3D single-layered graphene architecture with a large pore size and high surface area (>2000 m 2 g −1 ) sometimes collapses and reduces the structural regularity of the grown carbons during the template removal process using aqueous acids, as previously reported, 22 leading to stacked carbon layers.Hereaer, we focus on porous graphene analogs with a narrow pore distribution (<20 nm).

Zeolite-templated carbon (ZTC)
Zeolites are a class of inorganic materials composed of SiO 2 and Al 2 O 3 (aluminosilicates) with alkali metals as countercations.2][73][74][75][76] The catalytic ability and structural regularity of zeolites 77,78 are enticing features for their use as templates for synthesizing nanostructured carbon materials.In 2000, Kyotani and co-workers reported the synthesis of zeolite-templated carbon (ZTC) using Y zeolite (faujasite, FAU) as the template material. 11The studies used Y zeolite with a porous diamond-like framework of spherical cavities (supercage, ∼1.3 nm in diameter): 79 ZTC was prepared by transcription of the structural information of zeolites.A composite of furfuryl alcohol and Y zeolite powder was heated, followed by treatment with propylene at 600-800 °C for CVD to achieve the ordered porous structure of single-walled Fig. 1 Schematic of structurally well-defined graphene analogs with various dimensions of materials, including 3D graphene materials. 59ravimetric surface area of [60]fullerene is derived from the literature. 70anographene derivatives. 79Thermal annealing at 900 °C for 3 h ensures a more robust 3D structure. 79,80Aer CVD, the resulting material was washed with HF and HCl solutions to obtain the ZTCs.This procedure allowed the ZTC to retain the highly ordered microstructure of the zeolite with carbon architecture.
Ordered microporous structures provide a high surface area, large micropore volume, and fast diffusion rate of gases and electrolytes despite the narrow pore width.These features are suitable for gas physisorption 81 and electric double-layer capacitor 82 applications.The XRD pattern of the carbon material synthesized using Y zeolite as a template shows a peak at 2q = 6.26°, which corresponds to the 111 diffraction of the parent Y zeolite at 2q = 6.19°.This XRD pattern indicates that the original ordered structure of Y zeolite is maintained in the carbon material.The sharp diffraction peak indicates that the carbon material has excellent long-range order with a periodicity of 1.41 nm, which is the same as the 111 spacing of the Y zeolite.The adsorption isotherm shows a sharp increase in N 2 adsorption as P/P 0 increases in the low-pressure region and quickly reaches a plateau, indicating that the microporous structure exhibits a minimal number of mesopores or macropores.Both sides of the single-walled graphene-like ZTC surface can act as solid-liquid or solid-gas interfaces.In addition, edges also contribute to the surface area of ZTC, which reaches a gravimetric surface area (S g ) of >3000 m 2 g −1 .This feature enables efficient uptake of CH 4 (ref.26) and H 2 . 81orous carbon materials with the structural 3D regularity of the original parent material can also be synthesized by carbonization using other zeolites and inorganic nanomaterials.Acidity, as conrmed by pyridine-IR spectroscopy, plays an important role in controlling the quality of ZTCs. 83N-Doped 84,85 and B/N-doped 85 ordered carbon materials have also been prepared using zeolite-templated methods.They demonstrate the feasibility of the templating method for preparing ordered carbonaceous materials.

Nanoporous graphene (NPG)
2.2.1 Synthesis.The CVDs of gaseous unsaturated carbon sources with C^C triple bonds, such as acetylene, and C]C double bonds, such as propylene, have been investigated to prepare templated carbons. 11,87The resultant periodically arranged microstructured carbon cages enable efficient diffusion of gases and electrolytes. 23Typically incompatible high surface area, fast diffusion of gases and electrolytes, electrical conductivity, and structural exibility are realized using the templated method.However, control of uniform single-layer graphene growth is difficult, with signicant amounts of fragile oxygenrich edge sites being formed to reduce the chemical and electrochemical stability of the obtained carbon materials.
By contrast, aliphatic hydrocarbons such as CH 4 are relatively inert for carbon deposition reactions. 88It is expected that the efficient catalytic deposition of CH 4 on an ordered 3D template can achieve ideal 3D graphene with tailored microporosity.
Nanosized g-alumina is a promising template material for synthesizing nanoporous graphene (NPG) materials since it is one of the most efficient catalysts for catalytic C-H activation. 89H 4 -CVD takes place on alumina nanoparticles (ANPs) with the initial associative dissociation of CH 4 as the kinetic bottleneck, 59 and this is followed by acid etching and annealing 86,[90][91][92][93] to give NPGs as minimally stacked porous graphene analogs (Fig. 2).The resultant NPGs have a high surface area (>1800 m 2 (Bottom) Energy level diagrams of the initial CH 4 activation on the Al [6] site and Al [4] site of the g-Al 2 O 3 (100) surface during CH 4 -CVD for the synthesis of NPGs.59 g −1 ), high electric conductivity, elastic properties, and a spongelike mesoporous framework.
The use of inert CH 4 enabled us to selectively synthesize single-layered porous graphene materials.Density functional theory (DFT) calculations coupled with experimental kinetic analysis using thermogravimetry (TG) techniques revealed that the dehydration and subsequent surface activation of g-ANPs by CH 4 are crucial in controlling surface chemistry. 59According to the DFT calculations, the original octahedral site (Al [6] ) coordinated with six atoms of surrounding oxides affords a radical mechanism in the initial CH 4 activation, with an activation energy (DE ‡ ) of 270 kJ mol −1 .Further elimination of surface oxides eventually leads to more reactive tetrahedral sites (Al [4] ).The surface with oxygen vacancies provides a favorable reaction pathway for proton transfer (PT) reactions via the Lewis acid/ base mechanism, with a calculated apparent DE ‡ of 120 kJ mol −1 .This theoretical value agrees well with the experimental value of 124 kJ mol −1 obtained from the Arrhenius plot using the TG technique. 59This PT step is the kinetic bottleneck for the entire reaction.Subsequent PT results in the formation of surface methylene species ðCH * 2 Þ.DFT calculations also demonstrated that further carbon chain growth to form heavier aliphatic hydrocarbons by adding or inserting CH * 2 species is thermodynamically and kinetically feasible. 94q-ANPs are also applicable as template materials. 86,92o improve the efficiency of the synthesis and quality of the resultant NPGs and achieve ideal 3D graphene materials, it is essential to nd new templates that realize (i) efficient catalytic activation of CH 4 at lower reaction temperatures, (ii) better structural regularity of the resultant NPGs, and (iii) easy removal of the templates aer the CVD process.CH 4 -CVD on nanostructured oxides, including g-ANPs and zeolites, requires high temperatures above 800 °C for a sufficient rate of carbonization. 59Such a high temperature can easily damage the structural order over time. 101Fig. 3a shows the dependence of CH 4 partial pressure on the rate of CH 4 -CVD carbonization on g-ANPs.We found that the rate of carbonization decreased when the reaction reached the single-layer carbonization on g-ANPs.
Faster carbonization through better surface catalysis, as shown in Fig. 3b-1, is required to lower the reaction temperature and improve selectivity.Screening of catalysts using thermogravimetric analysis (TGA) is a promising approach.
The economical preparation of carbon materials is also important for practical applications. 102Template materials investigated to date, such as nanostructured silica, 103,104 g-ANPs, 59,86 q-ANPs, 92 and zeolite, 11 require the use of hazardous HF aqueous solutions for their removal aer CVD, which makes the synthetic process tedious.For practical industrial applications, HF should be replaced with the less hazardous HCl.Catalytically active MgO 105-107 is a promising template material 24,108,109 that does not require HF during template etching.Investigating the dissolution of ANPs and zeolites in benign and safe ways is crucial for the practical application of NPGs.
2.2.2 Structure.NPGs exhibit high surface area and very few edge sites.Table 1 summarizes the physicochemical properties of representative carbon materials.Another important feature of meso-structured elastic carbons is their highly exible carbon framework.The bulk modulus of NPG is less than 1 GPa, and this value is a magnitude smaller than those of typical "so" materials such as zeolite (14 GPa) and the relatively so class of metal-organic-frameworks (7.7 GPa). 99he surface area of NPGs mainly comprises the basal plane of single-layer graphene extended over the 3D nanospace instead of the edge sites. 92The surface area of NPGs obtained by using a g-ANP template reached 1800-2300 m 2 g −1 , and this lies between that of single-layered graphene (2627 m 2 g −1 ) and stacked bilayer graphene (1314 m 2 g −1 ). 59Temperatureprogrammed desorption (TPD) 8 of NPGs was investigated, and it showed much fewer edge sites on NPGs when compared with typical activated carbons and carbon black. 86,92The electrochemical stability of NPGs also conrms that the abovementioned structure has fewer terminal edge sites. 92he Raman spectra of NPGs indicate that they consist mostly of hexagonal aromatic rings, but some pentagons and

Chemical Science Review
heptagons exist, which introduce curvature to the NPGs in their grain boundaries. 86An intense G band at approximately 1587 cm −1 , as in typical graphene 110,111 (Fig. 2), coupled with a high specic surface area (S BET ∼2000 m 2 g −1 ) and a weak 002 diffraction in the XRD pattern indicate the presence of a singlelayered graphene structure in NPGs. 86The red-shied G ′ band at ∼2670 cm −1 , compared with that of typical graphite, 110,111 corroborates the presence of a single-walled graphene structure. 44,110The red-shied G ′ band may also reect the value of Young's moduli 96 by the introduction of curvature.In general, a relatively sharp D band (Fig. 2) in the Raman spectra can be mainly attributed to edges, 6,7 but TPD analysis indicates a very low occurrence of edges. 86,92Therefore, the prominent D band of the NPGs is mainly attributed to in-plane disorder instead of edges.
The type of disorder can be qualitatively analyzed using the intensity ratio between the D and D ′ bands, I D /I D ′. 112 The I D /I D ′ of NPGs is ca. 5.This indicates that these NPGs have both vacancies and grain boundaries since the I D /I D ′ values lie between those of graphene dominantly with vacancies (∼7) and grain boundaries (∼3.5). 112The shoulder peak at ∼1150 cm −1 in the Raman spectra proves the existence of Stone-Wales (SW) defects, 5,[112][113][114][115] while the small peak at ∼2460 cm −1 can be attributed to the SW + D band.
The mean distance between the defects R can be related to the intensity ratio of the D and G bands, I D /I G (R): 116 where r S = 1.00 nm is the mean radius of the structurally disordered region and r A = 3.00 nm is the mean radius of the activated region, where the graphitic structure is mostly conserved.However, its symmetry-breaking structure enhances the D band.C A = 4.2 and C S = 0.87 are parameters that describe the strength of the inuences of the structurally disordered and activated regions on the intensity of the D band, respectively. 116sed on this equation, the mean density of vacancy defects per hexagon of the graphene framework was 10 −2 for nanoporous carbons (NPCs) obtained by CH 4 -CVD and subsequent acid etching, whereas annealing of NPCs reduces the defect density to 10 −3 to afford the corresponding NPGs without any loss of porosity. 86he small peaks at ∼1150 cm −1 in the Raman spectra originate from heptagons and pentagons 5,113 in the grain boundaries 117 and surface defects 118,119 within continuous graphene-based materials 59,92 rather than edge sites.The domain boundary oen contains 5-and 7-membered rings, [3][4][5][117][118][119] which result in the curved structure shown in Fig. 4. Fig. 4 shows the geometries and molecular orbitals of nanographene models having a pentagon and heptagon as a structural defect. Both theHOMOs and LUMOs of the structural models were relatively localized around the edges of the curved nanographene structures, and the excellent chemical and electrochemical stability of the NPGs can be explained by the reduced presence of reactive edges, as conrmed by TPD analysis.92,100 3. Application of ordered porous graphene materials

Electric double-layer capacitors (EDLCs)
The most common application of highly ordered nanoporous carbon materials is electric double-layer capacitors (EDLCs): 1,39,100 EDLCs are extensively used in electric vehicles and other industrial elds.There are two important prerequisites for achieving efficient EDLCs.First, a high surface area of carbon materials is required to achieve EDLCs with high energy density, as S g and S v are directly related to the gravimetric and volumetric capacities, respectively. 120This can be realized by high porosity and small pore size because EDLCs can be charged in principle through the physisorption of electrolyte ions onto the nanopore surfaces of a carbon electrode. 120mportantly, this oen causes a lower efficiency of mass transportation within nanostructured materials because the ions have to be transferred from the outside into the porous architecture of the electrode materials before physisorption in the EDLCs can occur (Fig. 5). 40D structural regularity helps overcome these issues.For example, despite their microporous structure, ZTCs facilitate the efficient conveyance of ions under electrochemical conditions owing to their highly ordered architecture.This results in a high gravimetric capacitance of 140-190 F g −1 even at a high current of up to 20 A g −1 . 39,121Ideal 3D graphene materials with such structural regularity and a continuous graphene architecture will realize highly efficient EDLCs in terms of energy efficiency and stability.
Liu and co-workers used ZTCs with different pore sizes as theoretical models to study the effect of pore geometry on capacitance. 122According to their study, the charge compensation per carbon (CCpC) determines the capacitance, and a high CCpC tends to be related to a small radius of curvature of graphene.Tang and co-workers used NPGs with different graphene-stacking layers (the specic surface area changed accordingly) to explore the inuence of the specic surface area on the total capacitance and the origin of the total capacitance of 3D porous graphene. 1235][126][127][128][129] The critical factor for obtaining carbon materials with large capacitance is the presence of fewer graphene-stacking layers in the carbon frameworks with appropriate surface modication to ensure a large electrical double-layer capacitance.The ordered and well-dened structures of ideal 3D graphene materials are particularly interesting in exploring the origin of capacitance and methods to improve them further.

Next-generation Li-ion batteries
Since their rst introduction by the Sony Corporation in 1991, 130 lithium-ion batteries (LIBs) have been highly important energystorage techniques for use in mobile phones and electrical vehicles. 131For achieving the electrication of heavy-duty vehicles and aircra and storing solar energy in smart grids, developing much better secondary batteries with much higher specic energy will be necessary. 132Air-metal batteries, including Li-O 2 systems with Li-rich oxides as cathode materials, are promising candidates because of their high theoretical energy density. 1334][145][146] Ideally, 3D analogs of graphene materials would be suitable for achieving better electrical conductivity and supporting the reactants at the same time.
NPGs are promising scaffolds for novel LIBs because they have a high electron conductivity of up to 18 S cm −1 and excellent electrochemical stability owing to fewer reactive edge sites.NPGs also exhibit exibility with an extremely low bulk modulus of <1 GPa.NPGs with large pore volumes and exible nanopores have been applied as conductive additives in allsolid-state Li-S batteries, 92 with better electrochemical performance than MSC30-based cells.The 3D continuous graphene structure in the NPGs annealed at 1800 °C under an inert Fig. 5 Schematic of electric double-layer capacitor (EDLC) application of high-quality 3D continuous graphene materials.Edge sites are electrochemically reactive, 39 and therefore, NPGs with suppressed edges will be highly promising for EDLC applications.

Chemical Science Review
atmosphere results in higher electrochemical stability and better cycling. 86In addition, the nano-connement effect of insulating sulfur in conductive NPGs realizes durable threephase contact (Fig. 6). 92This strategy can also be applied to other batteries with different active materials.Tailor-made 3D ordered nanopores with an arbitrary pore size and structure provide improved nano-connement and clear-cut structureactivity relationships for better battery systems, including Li-O 2 systems, when coupled with catalytic centers 102,147,148 with better morphology for controlling cathode-electrolyte interaction 149 and electrochemical cycling.
Powder-type NPGs have the potential problem of grainboundary resistance and are difficult to handle.Pelletization of the template materials affords monolith-type NPGs aer CH 4 -CVD, thereby improving the connection of the grown nanographenes. 150

Refrigeration based on mechanical force
Efforts to achieve ideal 3D graphene materials would also be benecial for high-efficiency refrigeration systems.The introduction of curvature into single-layered graphene substantially reduces Young's modulus (Y).For example, the aforementioned ZTC and NPGs have a bulk modulus that is three orders of magnitude smaller than that of pristine single-layered graphene (Table 1).
We demonstrated that the nanopores of carbon materials could be reversibly deformed upon external pressurization up to 500 MPa and that the elastic properties are supported by quasilinear stress-strain curves with nearly no loss in energy.In the presence of water or alcohol vapor, the gas-liquid equilibrium is signicantly and compulsively altered upon deformation of the nanopores (Fig. 7a).This phenomenon could be used for refrigeration based on mechanical-force-induced phase transition of adsorbate (RMPTA) systems. 99NPGs with small Y values are a promising class of materials for RMPTA combined with water and alcohols as environmentally friendly adsorbates because the coefficient of performance (COP) is proportional to the reciprocal of the Young's modulus of the material (Y −1 ).Slow diffusion of molecules is a general issue related to the application of porous materials, 31,151 but ideal 3D graphene materials with structural regularity can achieve fast diffusion of gases and a more exible 3D continuous graphene structure simultaneously.
New ordered 3D NPG materials will realize better refrigeration systems based on the new operating principle with a uniform hierarchical structure (nm-to-mm scale) and resilience against deformation upon pressurization during the refrigeration cycle.A major impediment to efficient RMPTA systems is the uneven deformation of porous carbon materials under external pressurization.As shown in Fig. 7b, a sharp drop in temperature is observed during the compulsive liquid-gas phase transition upon pressurization, whereas nearly no heating is discernible despite the total recovery of the gas-phase pressure upon release.This irreversibility could be because of the lack of local structural robustness toward nonuniform stress.The uneven and irreversible structural changes in the nanopores are partly attributed to the structural heterogeneity of the NPGs owing to the inheritance of the irregular secondary particle structure appearing in their template materials, such as Al 2 O 3 and zeolites.Another issue is the low thermal   99 conductivity, and uniform nanographene growth in NPGs can also be achieved through improved CVD chemistry (Fig. 3b).

Conclusion and outlook
Since the proposal of Mackay crystals, several carbon materials have been reported to achieve high surface areas, structural regularity, and functionality.ZTCs are a class of carbon materials with a highly ordered 3D structure and a high specic surface area, while NPGs are extraordinary pluripotent materials with high electrochemical stability owing to fewer electrochemically active edges, a high electrical conductivity of up to 18 S cm −1 because of seamless and 3D-developed single graphene sheets, and highly exible mechanical structure with a bulk modulus of less than 1 GPa.We investigated a general strategy for synthesizing high-quality and continuous 3D nanographene materials using CH 4 -CVD on nanosized oxide surfaces, where the least stacking of nanographene was achieved to ensure a high surface area with suppressed edge sites.Further investigation will expand the scope of template materials, including ordered oxides 101,103 for synthesizing innovative 3D porous graphene materials in due course.However, challenges remain in achieving better homogeneity of nanographene growth and control of the hierarchical structure for better applications.As for 2D graphene growth, 153,154 better control of CVD chemistry by suitable surface catalysis 101,155 including well-controlled defects and dispersed metalcontaining reactive sites coupled with computational chemistry 156,157 will be crucial for better 3D graphene materials toward minimal surface graphene. 53,158comprehensive understanding of the structure of NPGs has been one of the central issues in this eld.Recent progress in the advanced characterization of carbon materials has accelerated our understanding and control of the nanostructure of advanced carbon materials.We addressed the qualication and quantication of surface defects in NPGs by TPD 86 and Raman spectroscopy, [159][160][161] whereas Poisson statistics are useful for quantitatively determining the distribution of graphene layers 86,[162][163][164] in continuous 3D graphenes.The complementary and convincing direct observation of defects by electron microscopy techniques 3,[165][166][167] will result in a much deeper understanding of the nanostructure.These insights into the atomic level structure of NPGs including the chemical and topological defects will be conducive to further control of highquality NPGs.Advanced characterization, including computational 168,169 and experimental (Raman spectroscopy, 86 angleresolved photoemission spectroscopy, 23,170 X-ray absorption ne structure spectroscopy, 171,172 electron energy loss spectroscopy, 173 X-ray photoelectron spectroscopy, 171 steady-state absorption spectroscopy, and neutron diffraction 174 ) approaches (Fig. 8), will provide a more sophisticated understanding and control of novel 3D graphene materials at the atomic level.
The successful application of NPGs and potential applications of ideal 3D graphene materials in supercapacitors, LIBs, and new refrigeration systems are also discussed in this review.Ideal 3D graphene materials will realize otherwise incompatible properties at the same time, namely, high electronic conductivity, ordered nanoporosity, exibility, and high chemical and electrochemical stability.The realization of structural regularity Fig. 8 Schematic of the integration of experimental results and computational chemistry, and modeling for molecular understanding of the obtained ordered porous 3D graphene materials.Various spectroscopic techniques are of interest for elucidating the structure at the atomic level in a self-consistent manner, including Raman spectroscopy, 86 angle-resolved photoemission spectroscopy, 23,170 X-ray absorption fine structure spectroscopy, 171,172 electron energy loss spectroscopy, 173 X-ray photoelectron spectroscopy, 171 steady-state absorption spectroscopy, and neutron diffraction. 174

Chemical Science Review
of NPGs can produce these features simultaneously, and it is anticipated that such unprecedented carbon materials will have new unexplored applications, including catalyst supports in gas-phase catalysis (for example, CO 2 hydrogenation 175 and CH 4 activation 73,78 ) as "hydrophobic analogs" of zeolites.A systematic investigation of tuned pore sizes 122,141 could also be considerably interesting for identifying otherwise hidden scientic aspects for many applications, including catalysis and batteries.Mechanical-force-induced changes in the nanopores of current NPGs (Fig. 7) occur nonuniformly because of the uneven structure of current carbon materials.Therefore, continued efforts to create ordered porous graphene materials with uniform hierarchical structures from the micro-to macroscale will help improve the efficiency of these applications.The combination of innovative synthesis, advanced characterization, and unexplored applications will open a new route for achieving more energy-efficient systems using next-generation NPGs.
Chemical Science Review

Fig. 2 (
Fig. 2 (Top) Schematic of the synthesis of nanoporous graphene materials via CH 4 -CVD 59 on Al 2 O 3 nanoparticles and their analysis 86 (reprinted with permission from ref. 86.Copyright 2023 Royal Society of Chemistry).(Bottom)Energy level diagrams of the initial CH 4 activation on the Al[6] site and Al[4] site of the g-Al 2 O 3 (100) surface during CH 4 -CVD for the synthesis of NPGs.59

Fig. 3
Fig. 3 (a) TGA of CH 4 -CVD on g-Al 2 O 3 nanoparticles at 900 °C with different partial pressures of CH 4 . 59(b) Expected ideal output of the TGA of CH 4 -CVD with enhanced surface catalysis for selective synthesis of single-layered porous graphene materials with improved integrity of "graphene nature".

Fig. 4
Fig.4Optimized geometries of nanographene models, and the corresponding Kohn-Sham highest molecular orbital (HOMO) and lowest molecular orbital (LUMO) obtained using the DFT method.

Fig. 6
Fig.6(a) Schematic of battery application of nanoporous graphene materials and (b) proposed degradation pathway which could be avoided by using the nano-confinement effect of NPGs 92 (reprinted with permission from ref.92.Copyright 2021 American Chemical Society).3D-ordered continuous graphene provides a precise structure-activity relationship, which is conducive to better understanding and control of applications.

Fig. 7
Fig.7(a) Schematic of a new refrigeration system based on the flexible deformation of ordered nanoporous graphene materials 152 upon pressurization,99 and (b) time-course of gas-phase pressure and temperature on the surface of the materials.99

Table 1
Summary of the physicochemical properties of materials Obtained from the DA plot.b V meso = V total − V micro .c Concentration of edge sites (N edge ) calculated by using TPD.d Bulk moduli (K), or otherwise, the calculated Young's modulus in parentheses.e At an applied pressure of 90 MPa.f Ideal values are shown in parentheses. a